Another explanation may be that the selected Au-NP was not actually an Au-NP but another nano-object with a height similar to that of the Au-NP. To further verify the attachment of the Au-NP to the probe, we examined TEM micrographs of the modified AFM probe, as shown in Figure 3. To facilitate selleck comparison, a new probe was also imaged. The original tip radius of curvature was verified as less
than 8 nm (Figure 3a). In a series of learn more experiments (using more than 50 AFM probes) and the same voltage pulse of 2 V for 32 ns, we were unable to observe Au-NPs on most of the AFM tips (Figure 3b), suggesting either that the Au atoms were distributed on the AFM tip without any particular structure or that they did not attach. In a few cases, we observed complete Au-NPs on the AFM tips in TEM micrographs; however, these Au-NPs appear to have been adsorbed on the AFM tips randomly  (see Additional file 1 for details). We then conducted conjugation experiments using 4-nm QDs to verify the existence of Au on these tips. TEM micrographs demonstrated that 44%
of the tips succeeded in picking up single QDs at the vertex (Figure 3c), while the remaining 56% did not (Figure 3d). Figure 3 TEM micrographs of the modified AFM probe. (a) TEM micrograph of the new AFM probe. (b) Following application of a 2-V pulse to the Au-NP for 32 ns, most of the probes presented no visible Au-NP. EPZ015938 After conjugating these probes with a QD, (c) 44% of tips were able to pick up single QDs (red arrow) and (d) 56% of tips were unable to pick up anything. Figure 4 illustrates the process of conjugating the Au-NP with QDs. HS(CH2)15COOH was first self-assembled on the Au atoms at the AFM tips to expose the carboxylic acid functional group (Figure 4a,b) for further QDs conjugation. Following activation by EDC and sulfo-NHS, an amine-reactive ester formed (Figure 4c,d). Finally, Qdot® ITK™ amino (PEG) QDs conjugated with the Au-NP through the formation of an amide bond. Figure 4 Process of conjugation between Au-NP and a 4-nm QD. (a,
b) HS(CH2)15COOH is first self-assembled on the Au atoms at the AFM tip to expose the carboxylic acid functional group. (c, d) Reaction with EDC and sulfo-NHS to form amine-reactive ester. (e) Attachment of functionalized Lck QDs by an amide bond. To verify the existence of a single QDs on the AFM tip, we monitored the fluorescence of single QDs using a far-field laser scanning confocal microscope. For comparison, we prepared half-glass and half-Au film (65 nm) substrates as reference samples (Figure 5). QDs samples were prepared by spin-coating a 0.1-nM solution of QD525 on the glass/Au film (65 nm) substrates. The root-mean-squared (RMS) value of the surface roughness on the Au film was estimated at less than 10 nm (see Additional file 1). The resulting emission trajectories are presented in Figure 6. Figure 5 Experimental setup for observation of fluorescence intensity in single QDs.